C 13 Planning resources for Sheet 93 1K-coating materials free of polyvinyl chloride and polyvinylidene chloride, low-solvent, also for repair (1K HS) General description of material: one-component coating material Binders: GB, ZB, DB: synthetic resins e.g. based on alkyd or acryl, free of polyvinyl chloride and polyvinylidene chloride Pigments: GB: corrosion protection pigments, inhibitors ZB and DB: micaceous iron oxide, tone pigments solid content (vol. %): GB, ZB and DB minimum 57 % Solvent content: GB maximum 23 %, ZB, DB maximum 25 % Thinner: substance No 693.150, maximum 3 % addition Additional notes: object temperature at least 5 °C and at least 3 K above dew point Table C 4.3.13: Planning resources for materials according to Sheet 93 Area of application Protective system Application Minimum waiting time before System structure Surface Nominal dry film subsequent preparation thicknesses [μm] coating at approx. 20 °C dry wet - initial protection GB: 1. GB Sa 2½ 80 140 spraying, 16 h spreading 1K HS-active - full renewal on the pigment subst. No construction site 693.01/02 80 140 2nd GB and/or edge protection No 693.06 2K-EP-zinc dust Sa 2½ 70 100 spraying No 687.03/04/05 zinc spraying Sa 3 100 spraying none hot dip galvanising as Be ) hot dipping none per DIN EN ISO 1461)) ZB: 1K HS-EG No clean 80-120 140-190 spraying, 16 h 693.12 to 693.14) depending on spreading the surface condition and DB: 1K HS-EG subst. 80-120 140-190 spraying, dirt No 693.30 to spreading, 693.74) rolling6) 1K HS No 693.80 to 693.99) (colour tones according to RAL) continued on next page Substances according to Sheet 93 are not suitable: for high mechanical stress, − for chemical stress, − for hot dip galvanising without pre-treatment. −
C 13 Planning resources for Sheet 93 1K-coating materials free of polyvinyl chloride and polyvinylidene chloride, low-solvent, also for repair (1K HS) General description of material: one-component coating material Binders: GB, ZB, DB: synthetic resins e.g. based on alkyd or acryl, free of polyvinyl chloride and polyvinylidene chloride Pigments: GB: corrosion protection pigments, inhibitors ZB and DB: micaceous iron oxide, tone pigments solid content (vol. %): GB, ZB and DB minimum 57 % Solvent content: GB maximum 23 %, ZB, DB maximum 25 % Thinner: substance No 693.150, maximum 3 % addition Additional notes: object temperature at least 5 °C and at least 3 K above dew point Table C 4.3.13: Planning resources for materials according to Sheet 93 Area of application Protective system Application Minimum waiting time before subsequent coating at approx. 20 °C System structure Surface preparation Nominal dry film thicknesses [μm] dry wet - initial protection - full renewal on the construction site GB: 1. GB 1K HS-active pigment subst. No 693.01/02 2nd GB and/or edge protection No 693.06 Sa 2½ 80 140 spraying, spreading 16 h 80 140 2K-EP-zinc dust No 687.03/04/05 Sa 2½ 70 100 spraying zinc spraying Sa 3 100 spraying none hot dip galvanising as per DIN EN ISO 1461)) Be ) hot dipping none ZB: 1K HS-EG No 693.12 to 693.14) clean depending on the surface condition and dirt 80-120 140-190 spraying, spreading 16 h DB: 1K HS-EG subst. No 693.30 to 693.74) 1K HS No 693.80 to 693.99) (colour tones according to RAL) 80-120 140-190 spraying, spreading, rolling6) continued on next page Substances according to Sheet 93 are not suitable: − for high mechanical stress, − for chemical stress, − for hot dip galvanising without pre-treatment.
text_2011_0574_D.docx